DIN EN 10297-1 (06/2003) Welded circular steel pipes for machine construction and general technical service stainless steel.Pipes made from stainless and alloy steel:SEW 310 (08/1992) physical properties of steel:VdTÜV / Werkstoffblatt 147 /Ausgbe 09.01:rolled and forged steel 42CrMo4, Material-Nr. 1.7225 1.7225 / 42CrMo4 - Qualitätsstahl - Akrostal - StahlhandelMechanical properties of a product with diameter d 16 mm:Property:Designation:Unit:After heat treatment:Ultimate tensile strength:R m:MPa:1100-1300:Yield stress:R e (R p0,2) MPa 900:Elongation:A % 10:Reduction of area:Z % 40:Impact energy:KV:J 30:Effect of the cross-section on mechanical properties
AISI 4140 Steel Bar, Steel Plate, Flats Supplier, Stockist and Exporter. AISI SAE 4140 alloy steel is a chromium molybdenum alloy steel specification widely used in general purpose high tensile steel for components, like axles, shafts, bolts, gears and other applications. Similar to alloy grade AISI 4130 chrome moly alloy steel but with a slightly higher 42CRMO4 (+QT) - MEKA SteelGrade 42CRMO4 (+QT) According EN 10083 -3 ISO 683 -17 Article code 429.13.92.08 WN 1.7225 Standards & Specifications Version 01/02.11.2013 Page s 02 04-02 Product Standards Material Specification Quality Standards Project CMT coop MCI (DRT) Author AKa Source SKF 1 GENERAL 42CrMo4 - Ovako42CrMo4 is a steel for quenching and tempering, which has a good combination of strength and toughness in the quenched and tempered condition. After the oil quenching, the steel will be through hardened up to ø60 mm bar diameter. The microstructure of larger dimensions is not fully martensite. The steel is applicable to induction hardening.
42CrMo4 - 1% Chromium-Molybdenum Through Hardening Steel Surcharge The surcharge information provided is a guide to market scrap and alloy surcharges and is an averaged value taken from various suppliers surcharge mechanisms and isnt therefore necessarily the surcharge applied to 42CrMo4 steel round 42CrMo4 forging steel 42CrMo4 42CrMo4 is an engineering alloy steel containing chromium and molybdenum. It falls in a class of low alloy steel. It has high fatigue strength, abrasion and impact resistance, toughness, and torsional strength. It can be heat treated in a number of ways to give it a superior combination of properties. We can provide you 42CrMo4 in the following forms 42CrMo4 |42CrMoS4|1.7225 - Xingsheng Special steelaisi 1045 1.1191 c45 s45c; aisi 4130 1.7218 25crmo4 scm430; aisi 4140 1.7225 42crmo4 scm440; aisi 4340 1.6511 36crnimo4 sncm439
42CrMo4, 1.7225, 42CrMoS4, 1.7227, AISI 4140 description. Structural steel, strong and hardenable. With this steel one can achieve very good properties on the whole cross-section (while quenching in oil, the max diameter is 70mm, for quenching in water it is 50mm). In the surface hardened condition in achieves a hardness of 54-59 HRC on the surface. 42crmo mechanical properties - Carbon steels - Q235 Mild 1.7225 Material 42CrMo4+QT Steel Chemical Composition . 42CrMo4+QT Introduction. 42CrMo4 material is an alloy steel, the delivery status of 42CrMo4 is mostly tempered (+ QT is short for quenched and tempered), it has high strength, high toughness, good hardenability, temper brittleness, high fatigue limit, good impact resistance after quenching and tempering, and good low temperature impact BS EN 42CrMo4 1.7225 Alloy Engineering Steel - QiLu Although 42CrMo4 steel is more expensive than 41Cr4 steel, it is more preferable in terms of material properties. EN 42CrMo4 alloy engineering steel materials have been widely used in automotive driving elements. Otai Steel is able to supply you prime quality of 42CrMo4 alloy steel materials with wide range. 1.42CrMo4 Alloy Steel Supply Range
The 42CrMo4 alloy material also has high fatigue strength and good low-temperature impact toughness. The temper brittleness is not obvious. Although 42CrMo4 steel is more expensive than 41Cr4 steel, it is more preferable in terms of material properties. EN 42CrMo4 alloy engineering steel materials have been widely used in automotive driving elements. DIN 1.7225 / AISI 4140 alloy structure steel1.7225 is a chromium molybdenum alloy steel specification widely used in the oil and gas industry. Similar to grade AISI 4130 but with a slightly higher carbon content. The higher carbon content of AISI 4140 gives greater strength and heat treatment capabilities in comparison to AISI 4130, however it does have inferior weldability characteristics. DIN 42CrMo4 - Equivalent MaterialsEN 42CrMo4 EN 1.7225:GOST 42HM:GB ML42CrMo:UNS G41400:Equivalent Materials Terms and Conditions. Overall statistics about our Database. 5184 Equivalencies. 13 Standard Organizations. Click below to see material properties of DIN 42CrMo4 on Matmatch.
1.7225 42CrMo4 M4S Chemical composition:C Cr Mo (Typical analysis in %) 0,42 1,10 0,25 Steel properties:CrMo-alloyed steel, engineering steel supplied in quenched and tempered conditions. Good machinability. Applications:Components with high requirements on toughness, e.g. gear wheels, pinions, connecting rods, parts for Quality 42CrMo4 /XFHILQ *URXS42CrMo4 1.7225 Data under fatigue +20 °C +N 328 Cyclic yield strength, y· N/mm2 low cycle number +QT 716 +N 0.12 Cyclic strength exponent, n low cycle number +QT 0.10 +N 673 Cyclic strength coefficient, K · N/mm2 low cycle number +QT 1367 +N 1000 )atigue strength coefficient, f · N/mm2 low cycle number +QT 1454 SIQUAL 7225 SteelSIQUAL 7225 Steel Designation by Standards Brand Name Ravne Mat. No. DIN EN AISI/SAE SIQUAL 7225 VCMO140 1.7225 - 42CrMo4 4142 Chemical Composition (in weight %) C Si Mn Cr Mo Ni V W Others 0.41 0.20 0.75 1.05 0.23 - - - - Description
42CrMo4 material (1.7225 steel) is an European standard alloy steel, the delivery condition of this steel is mostly tempered and quenched, it has high strength, high toughness, good hardenability, temper brittleness, high fatigue limit, good impact resistance after quenching and tempering, and good low temperature impact toughness. This steel is suitable for the manufacture of large and medium-sized
Please Click here